- Nano Express
- Open Access
Photocurrent response and semiconductor characteristics of Ce-Ce2O3-CeO2-modified TiO2 nanotube arrays
© Tan et al.; licensee Springer. 2014
Received: 12 September 2013
Accepted: 2 February 2014
Published: 10 February 2014
We reported Ce and its oxide-modified TiO2 nanotube arrays (TNTs) and their semiconductor properties. The TNTs were prepared by anodic oxidation on pure Ti and investigated by electrochemical photocurrent response analysis. Then, the TNT electrodes were deposited of Ce by cathodic reduction of Ce(NO3)3 6H2O. After deposition, the TNT electrodes were fabricated by anodic oxidation at E = 1.0 V(SCE) for various electricity as Ce-Ce2O3-CeO2 modification. The Ce-deposited TNTs (band gap energy Eg = 2.92 eV) exhibited enhanced photocurrent responses under visible light region and indicated more negative flat band potential (Efb) compared with the TNTs without deposition. After anodic oxidation, the mixed Ce and its oxide (Ce2O3-CeO2)-modified TNT photoelectrodes exhibited higher photocurrent responses under both visible and UV light regions than the TNTs without deposition. The photocurrent responses and Efb were found to be strongly dependent on the contents of Ce2O3 and CeO2 deposited on TNTs. A new characteristic of Eg = 2.1 ± 0.1 eV was investigated in the Ce2O3- and CeO2-modified photoelectrodes. X-ray diffraction (XRD), scanning electron microscopy (SEM), and X-ray photoelectron spectroscopy (XPS) were also employed to characterize various modified TNTs photoelectrodes.
One-dimensional TiO2 nanotubes arrays (TNTs) can provide higher surface area  and higher interfacial electricity transfer rate rather than spherical particles . TNTs have been modified by deposition of metal or metal oxides [3, 4] to indicate an enhanced photoelectric response under visible light. Nowadays, the rare earth metal Ce with f electron distribution has received extensive attention  for its energy levels located in the forbidden band of TiO2 which can form additional levels to accelerate the separation of electrons and holes . The different electronic structures of Ce3+ with 4f15d0 and Ce4+ with 4f05d0 indicate different optical properties [7–10]. The oxides of Ce indicate different semiconductor characteristics such as Ce2O3, with narrow bandgap energy (Eg = 2.4 eV), which is able to absorb visible light and CeO2, with wide bandgap energy (Eg = 3.16 eV), which can strongly absorb UV light even better than TiO2. The redox couple of Ce3+/Ce4+ can shift between CeO2 and Ce2O3 during oxidizing and reducing process . Li et al.  reported higher adsorption equilibrium constant and higher separation efficiency of electron-hole pairs obtained simultaneously from Ce3+-TiO2 catalysts. Due to the less acknowledgement of behavior of Ce and its oxides, the researches about Ce and its oxide deposition on TNTs are uncommon.
In this study, different proportions of Ce mixtures (Ce, CeO2, and Ce2O3) deposited TNTs were prepared to investigate their photocurrent responses and semiconductor characteristics.
Prior to anodization, the titanium sheets were mechanically polished with different abrasive papers and ultrasonically degreased in acetone and ethanol, respectively, finally rinsed with deionized water and dried in air. All the anodization experiments were carried out in a conventional two-electrode electrochemical cell under magnetic agitation condition at room temperature, with titanium foil as the anode and platinum foil as the cathode. The ethylene glycol solution containing 0.5 wt.% NH4F and 1.5 vol% H2O was used as electrolyte. The anodization voltage was constant at 20 V with a direct current power supply. The anodization process was performed for 6 h to obtain TNTs. After electrochemical anodization, the as-anodized TNTs were immediately rinsed with deionized water and then dried at 100°C. All samples were annealed at 450°C for 1.5 h to transform amorphous TiO2 to crystalline phase.
Firstly, the reductive Ce-deposited TNTs were performed by electrochemical reduction. The as-prepared TNTs with exposed area 0.2826 cm2 were inserted in 0.01 M Ce(NO)3 · 6H2O alcohol electrolyte for 1 h adsorption. Then, the above TNTs were used as working electrode, a Pt foil as the anode, and a saturated calomel electrode (SCE) as the reference electrode in the electrolyte. A potential E = -6 V was applied in the three-electrode system until a total electricity Q = 0.01 C to reduce Ce3+ into elemental Ce deposition on TNTs. This modified sample was named as TNTs-Ce. Secondly, several TNTs-Ce samples were oxidized by potentiostat powered by an anodic potential E = 1.0 V to the sample in supporting electrolyte (0.01 M Ce(NO3)3) for total electricity Q = 0.00001, 0.00025, 0.005, and 0.01 C, respectively. The oxidized samples were denoted as TNTs-0.00001 C, TNTs-0.00025 C, TNTs-0.005 C, and TNTs-0.01 C, correspondingly.
The morphologies were observed using field emission scanning electron microscope (FE-SEM, JSM-7500 F) with energy dispersive X-ray spectroscopy (EDX). The crystal phases and composition were characterized by X-ray diffraction (XRD, Y-2000) and X-ray photoelectron spectroscopy (XPS, MT-500, with Al monochromator with C1s at 284.8 eV). The photocurrent response measurements were carried out in an improved three-electrode electrochemical cell with a quartz window and 0.1 M Na2SO4 as supporting electrolyte. A 450-W Xeon lamp, a CT110 monochromator (1/8, Crowntech), and a potentiostat (PARSTAT2273, Princeton Applied Research, Oak Ridge, TN, USA) were also applied for electrochemistry measurements. The Mott-Schottky plots were performed with frequency 1,000 Hz and applied potential from -1.0 to 0.5 V by 0.1 V steps.
Results and discussion
Ratio of Ce in various photoelectrodes calculated from XPS analysis
where I0, hv, Eg, A, and n are fully discussed in  and n = 2 for the indirect transition of semiconductors. Figure 3B shows the photocurrent responses vs. photon energy plots for TNTs with various Ce deposits. Based on linear fitting, the characteristic Eg of various photoelectrodes can be derived respectively. Eg of the TNTs-Ce is reduced to 2.92 eV. After anodic oxidation, all the samples are located in the Eg between 3.0 to 3.1 eV, which are smaller than Eg of TNTs (3.15 eV) as a result of simple substance Ce existence.
Figure 3C shows the details of low electron energy part of Figure 3B. The various Ce-deposited TNTs indicated Eg of 2.1 ± 0.1 eV which is close to the Eg = 2.4 eV of Ce2O3. And these differences may be caused by the deposition of the simple substance Ce.
Flat band potentials calculated from Mott-Schottky plots
Ce-modified TNTs indicated stronger photocurrent response in visible light and less noble flat band potential than TNTs. After anodic oxidation, the Ce-Ce2O3-CeO2-modified TiO2 nanotube arrays indicated higher photocurrent responses in both visible and UV light region. As the anodic oxidation in depth with Ce2O3 and CeO2 was increasing, the photocurrent responses reinforced, but the flat band potential moved to noble potential comparing to the TNTs-Ce. A characteristic Eg = 2.1 ± 0.1 eV in line with Ce2O3 was discovered from the photocurrent responses which increased the photocurrent responses in visible light region.
This work is supported by the Fundamental Research Funds for the Central Universities (13MS80).
- Poulomi R, Steffen B, Patrik S: TiO2 Nanotubes: synthesis and applications. Synth Appl 2011, 50: 2904–2939.Google Scholar
- Jennings JR, Ghicov A, Peter LM, Schmuki P, Walker AB: Dye-sensitized solar cells based on oriented TiO2 nanotube arrays: transport, trapping, and transfer of electrons. J Am Chem Soc 2008, 130: 13364–13372. 10.1021/ja804852zView ArticleGoogle Scholar
- Lingjuan L, Jun L, Guangqing X, Yan W, Kui X, Zhong C, Yucheng W: Uniformly dispersed CdS nanoparticles sensitized TiO2 nanotube arrays with enhanced visible-light photocatalytic activity and stability. J Solid State Chem 2013, 208: 27–34.View ArticleGoogle Scholar
- Shiping X, Alan JD, Jincheng L, Jiawei N, Darren DS: Highly efficient CuO incorporated TiO2 nanotube photocatalyst for hydrogen production from water. Int J Hydrogen Energy 2011, 36: 6560–6568. 10.1016/j.ijhydene.2011.02.103View ArticleGoogle Scholar
- Zhang YN, Zhao GH, Lei YZ, Wu ZY, Jin YN, Li MF: Novel construction of CdS-encapsulated TiO2 nano test tubes corked with ZnO nanorods. Mater Lett 2010, 64: 2194–2196. 10.1016/j.matlet.2010.07.013View ArticleGoogle Scholar
- Chen JT, Li XJ, Yang Y, Wang LY, He MX: Effect of Re doping for photocatalytic properties of TiO2 thin films. J Chin Rare Earth Soc 2003, 21: 67–70.Google Scholar
- Orera VM, Merino RI, Pena F: Ce3+ ↔ Ce4+ conversion in ceria-doped zirconia single crystals induced by oxido-reduction treatments. Solid State Ion 1994, 72: 224–231.View ArticleGoogle Scholar
- Yen WM, Raukas M, Basun SA, Schaik WV, Happek U: Optical and photoconductive properties of cerium-doped crystalline solids. J Luminesc 1996, 69: 287–294. 10.1016/S0022-2313(96)00107-XView ArticleGoogle Scholar
- Gratian RB, Takashi U, Yoshimoto A, Kazuhiro S, Hironori A: The photocatalytic oxidation of water to O2 over pure CeO2, WO3, and TiO2 using Fe3+ and Ce4+ as electron acceptors. Appl Catal, A 2001, 205: 117–128. 10.1016/S0926-860X(00)00549-4View ArticleGoogle Scholar
- Ryuhei N, Akihiro O, Hitoshi O, Hiroshi I, Kazuhito H: Design of all-inorganic molecular-based photocatalysts sensitive to visible light: Ti(IV)–O - Ce(III) bimetallic assemblies on mesoporous silica. J Am Chem Soc 2007, 129: 9596–9597. 10.1021/ja073668nView ArticleGoogle Scholar
- Zou YL, Li Y, Guo Y, Liu XL, Cai H, Li JG: Study on the photoluminescence of nano-CeO2. J Liaoning Norm Univ (Nat Sci Edit) 2009, 32: 212–214.Google Scholar
- Chen QF, Jiang D, Xu Y, Wu D, Sun YH: Visible region photocatalysis of Ce-Si/TiO2 synthesized using sol–gel-hydrothermal method. Acta Phys -Chim Sin 2009, 25: 617–623.Google Scholar
- Li FB, Li XZ, Hou MF, Cheah KW, Choy WCH: Enhanced photocatalytic activity of Ce3+–TiO2 for 2-mercaptobenzothiazole degradation in aqueous suspension for odour control. Appl Catal A 2005, 285: 181–189. 10.1016/j.apcata.2005.02.025View ArticleGoogle Scholar
- Luo L PhD Thesis. In Study on surface oxidation of cerium metal by Xps. China: Academy of Engineering Physics; 2005.Google Scholar
- Mott NF, Davis EA: Electronic Processes in Non-Crystalline Materials. 2nd edition. Oxford: Clarendon Press; 1979.Google Scholar
- Kontos AI, Likodimos V, Stergiopoulos T, Tsoukleris DS, Falaras P: Self-organized anodic TiO2 nanotube arrays functionalized by iron oxide nanoparticles. Chem Mater 2009, 21: 662–672. 10.1021/cm802495pView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.